Output from "TOTOPOL", (version 1.92, 17 Jul 2017, Mike Treacy).

Report for the framework in file "public/tmp/tmp_194_6_110381979_7kHHxP.cif"

There are 144 T-atoms per unit cell
There are 288 O-atoms per unit cell

Framework density = 23.73 T-atoms per nm^3
Material density = 2.368 grams per cm^3 (excluding extra-framework material)
-------------------------------------------------------------------
-------------------------- T-O Analysis ---------------------------
-------------------------------------------------------------------
[Si] Ideal SiO distance = 1.610 Angstrom
T1  -- O1  = 1.5588 Angstrom
T1  -- O2  = 1.6466 Angstrom
T1  -- O3  = 1.6680 Angstrom
T1  -- O4  = 1.6749 Angstrom
      mean = 1.6371 Angstrom
        t1 = 0.061365  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.044801  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T2  -- O4  = 1.7041 Angstrom
T2  -- O5  = 1.6747 Angstrom
T2  -- O6  = 1.6146 Angstrom
T2  -- O7  = 1.6608 Angstrom
      mean = 1.6635 Angstrom
        t1 = 0.076189  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.056848  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T3  -- O6  = 1.6651 Angstrom
T3  -- O8  = 1.6697 Angstrom
T3  -- O9  = 1.7662 Angstrom
T3  -- O10 = 1.6475 Angstrom
      mean = 1.6871 Angstrom
        t1 = 0.071276  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.032635  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T4  -- O7  = 1.6770 Angstrom
T4  -- O9  = 1.7765 Angstrom
T4  -- O11 = 1.6216 Angstrom
T4  -- O12 = 1.6243 Angstrom
      mean = 1.6749 Angstrom
        t1 = 0.068042  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.041678  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T5  -- O10 = 1.6423 Angstrom
T5  -- O13 = 1.6518 Angstrom
T5  -- O14 = 1.5773 Angstrom
T5  -- O15 = 1.6085 Angstrom
      mean = 1.6200 Angstrom
        t1 = 0.040043  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.035791  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T6  -- O15 = 1.6278 Angstrom
T6  -- O16 = 1.6010 Angstrom
T6  -- O17 = 1.6314 Angstrom
T6  -- O18 = 1.6095 Angstrom
      mean = 1.6174 Angstrom
        t1 = 0.016142  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.022430  (0.0 is a perfect tetrahedron)

        T-O SUMMARY
          Range  = 1.5588 A <--> 1.7765 A
          Mean   = 1.6500 A
          StdDev = 0.0494 A

       t1 Range  = 0.0161 <-- 0.0555 --> 0.0762
       t2 Range  = 0.0224 <-- 0.0390 --> 0.0568

-------------------------------------------------------------------
------------------------- O-T-O Analysis --------------------------
-------------------------------------------------------------------
O1  -- T1  -- O2  = 103.027 deg; O1  -- O2  = 3 A
O1  -- T1  -- O3  = 104.887 deg; O1  -- O3  = 3 A
O1  -- T1  -- O4  =  98.922 deg; O1  -- O4  = 2 A
O2  -- T1  -- O3  = 113.572 deg; O2  -- O3  = 3 A
O2  -- T1  -- O4  = 115.079 deg; O2  -- O4  = 3 A
O3  -- T1  -- O4  = 118.180 deg; O3  -- O4  = 3 A
       98.922 deg <-- 108.944 deg --> 118.180 deg

O4  -- T2  -- O5  = 124.721 deg; O4  -- O5  = 3 A
O4  -- T2  -- O6  = 100.298 deg; O4  -- O6  = 3 A
O4  -- T2  -- O7  = 105.771 deg; O4  -- O7  = 3 A
O5  -- T2  -- O6  =  95.050 deg; O5  -- O6  = 2 A
O5  -- T2  -- O7  = 111.674 deg; O5  -- O7  = 3 A
O6  -- T2  -- O7  = 119.567 deg; O6  -- O7  = 3 A
       95.050 deg <-- 109.514 deg --> 124.721 deg

O6  -- T3  -- O8  = 103.810 deg; O6  -- O8  = 3 A
O6  -- T3  -- O9  = 106.079 deg; O6  -- O9  = 3 A
O6  -- T3  -- O10 = 114.563 deg; O6  -- O10 = 3 A
O8  -- T3  -- O9  = 122.887 deg; O8  -- O9  = 3 A
O8  -- T3  -- O10 = 101.763 deg; O8  -- O10 = 3 A
O9  -- T3  -- O10 = 108.117 deg; O9  -- O10 = 3 A
       101.763 deg <-- 109.536 deg --> 122.887 deg

O7  -- T4  -- O9  = 123.144 deg; O7  -- O9  = 3 A
O7  -- T4  -- O11 = 105.575 deg; O7  -- O11 = 3 A
O7  -- T4  -- O12 = 105.200 deg; O7  -- O12 = 3 A
O9  -- T4  -- O11 = 107.255 deg; O9  -- O11 = 3 A
O9  -- T4  -- O12 = 107.500 deg; O9  -- O12 = 3 A
O11 -- T4  -- O12 = 107.304 deg; O11 -- O12 = 3 A
       105.200 deg <-- 109.330 deg --> 123.144 deg

O10 -- T5  -- O13 = 118.813 deg; O10 -- O13 = 3 A
O10 -- T5  -- O14 = 103.806 deg; O10 -- O14 = 3 A
O10 -- T5  -- O15 = 109.748 deg; O10 -- O15 = 3 A
O13 -- T5  -- O14 = 107.013 deg; O13 -- O14 = 3 A
O13 -- T5  -- O15 = 111.051 deg; O13 -- O15 = 3 A
O14 -- T5  -- O15 = 105.265 deg; O14 -- O15 = 3 A
       103.806 deg <-- 109.283 deg --> 118.813 deg

O15 -- T6  -- O16 = 107.254 deg; O15 -- O16 = 3 A
O15 -- T6  -- O17 = 113.463 deg; O15 -- O17 = 3 A
O15 -- T6  -- O18 = 109.147 deg; O15 -- O18 = 3 A
O16 -- T6  -- O17 = 108.494 deg; O16 -- O17 = 3 A
O16 -- T6  -- O18 = 108.858 deg; O16 -- O18 = 3 A
O17 -- T6  -- O18 = 109.515 deg; O17 -- O18 = 3 A
       107.254 deg <-- 109.455 deg --> 113.463 deg

        O-T-O SUMMARY
          Range  = 95.0504 deg <--> 124.7210 deg
          Mean   = 109.5324 deg
          StdDev = 7.0972 deg

        O--O SUMMARY
          Range  = 2.4264 A <--> 3.0375 A
          Mean   = 2.6978 A
          StdDev = 0.1485 A

-------------------------------------------------------------------
------------------------- T-T-T Analysis --------------------------
-------------------------------------------------------------------
-------------------------------------------------------------------
------------------------- T-O-T Analysis --------------------------
-------------------------------------------------------------------
T1  -- O1  -- T1  = 141.903 deg ; T1  -- T1   2.9470 A

T1  -- O2  -- T1  = 126.718 deg ; T1  -- T1   2.9437 A

T1  -- O3  -- T1  = 126.063 deg ; T1  -- T1   2.9731 A

T1  -- O4  -- T2  = 171.201 deg ; T1  -- T2   3.3690 A

T2  -- O5  -- T2  = 121.474 deg ; T2  -- T2   2.9220 A

T2  -- O6  -- T3  = 108.864 deg ; T2  -- T3   2.6680 A

T2  -- O7  -- T4  = 157.056 deg ; T2  -- T4   3.2711 A

T3  -- O8  -- T3  = 116.226 deg ; T3  -- T3   2.8354 A

T3  -- O9  -- T4  = 150.165 deg ; T3  -- T4   3.4233 A

T3  -- O10 -- T5  = 126.043 deg ; T3  -- T5   2.9318 A

T4  -- O11 -- T4  = 139.045 deg ; T4  -- T4   3.0383 A

T4  -- O12 -- T4  = 143.656 deg ; T4  -- T4   3.0866 A

T5  -- O13 -- T5  = 120.152 deg ; T5  -- T5   2.8632 A

T5  -- O14 -- T5  = 148.840 deg ; T5  -- T5   3.0388 A

T5  -- O15 -- T6  = 119.679 deg ; T5  -- T6   2.7982 A

T6  -- O16 -- T6  = 156.139 deg ; T6  -- T6   3.1328 A

T6  -- O17 -- T6  = 130.228 deg ; T6  -- T6   2.9599 A

T6  -- O18 -- T6  = 130.626 deg ; T6  -- T6   2.9249 A


        T-O-T SUMMARY
          Range  = 108.8644° <--> 171.2009 deg
          Mean   = 135.2265 deg
          StdDev = 16.2595 deg

        T--T SUMMARY
          Range  = 2.6680 A <--> 3.4233 A
          Mean   = 3.0071 A
          StdDev = 0.1884 A

-------------------------------------------------------------------
------------------------ *** WARNINGS *** -------------------------
-------------------------------------------------------------------

T-T-T analysis was not conducted.

SOME T-ATOM DISTANCES ARE OUTSIDE THE NORMAL RANGE
T1  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T1  -- T1  = 2.9437 Angstrom
  T1  -- T2  = 3.3690 Angstrom
  T1  -- T3  = 3.4640 Angstrom
  T1  -- T1  = 2.9731 Angstrom
  T1  -- T1  = 2.9470 Angstrom
T2  has 6 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T2  -- T1  = 3.3690 Angstrom
  T2  -- T2  = 2.9220 Angstrom
  T2  -- T3  = 2.6680 Angstrom
  T2  -- T4  = 3.1673 Angstrom
  T2  -- T2  = 2.8608 Angstrom
  T2  -- T4  = 3.2711 Angstrom
T3  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T3  -- T1  = 3.4640 Angstrom
  T3  -- T2  = 2.6680 Angstrom
  T3  -- T3  = 2.8354 Angstrom
  T3  -- T4  = 3.4233 Angstrom
  T3  -- T5  = 2.9318 Angstrom
T4  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T4  -- T2  = 3.1673 Angstrom
  T4  -- T3  = 3.4233 Angstrom
  T4  -- T4  = 3.0383 Angstrom
  T4  -- T4  = 3.0866 Angstrom
  T4  -- T2  = 3.2711 Angstrom
T5  -- T6  = 2.7982 Angstrom
T6  -- T5  = 2.7982 Angstrom

-------------------------------------------------------------------
---------------------- Topological Analysis -----------------------
-------------------------------------------------------------------
T1 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 20 35 58 89 125 166 213 268 329 390 453 527 618 716
TD10 = 989
Circuit symbol = 4.6_{2}.4.8_{6}.6_{2}.6_{2}
Weight = 24
Vertex symbol  = 4.6_{2}.4.8_{4}.6.6_{2}
Weight = 24

T2 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 24 42 65 95 135 182 229 276 330 397 476 559 635 711
TD10 = 1064
Circuit symbol = 4.6_{2}.6_{2}.6_{2}.6_{2}.8_{6}
Weight = 22
Vertex symbol  = 4.6_{2}.6_{2}.6_{2}.6_{2}.8_{3}
Weight = 22

T3 (Si): multiplicity = 24
Coordination Sequence =
    1 4 12 25 41 64 94 131 178 229 279 333 396 471 554 635 716
TD10 = 1058
Circuit symbol = 6.6_{2}.6.8_{4}.6_{3}.8
Weight = 25
Vertex symbol  = 6.6_{2}.6.8_{2}.6_{3}.8
Weight = 25

T4 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 24 44 71 103 140 181 225 276 337 407 481 555 632 715
TD10 = 1080
Circuit symbol = 4.8_{5}.6.6_{2}.6_{2}.6_{2}
Weight = 27
Vertex symbol  = 4.8_{3}.6.6_{2}.6_{2}.6_{2}
Weight = 27

T5 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 19 37 60 86 119 162 215 276 338 396 456 530 622 721
TD10 = 988
Circuit symbol = 4.6_{2}.4.8_{3}.4.8_{3}
Weight = 22
Vertex symbol  = 4.6_{2}.4.8.4.8
Weight = 22

T6 (Si): multiplicity = 24
Coordination Sequence =
    1 4 8 13 23 44 78 120 164 209 259 319 389 463 535 606 685
TD10 = 923
Circuit symbol = 4.4.4.6.4.6_{2}
Weight = 12
Vertex symbol  = 4.4.4.6.4.8
Weight = 17

<TD10> = 1017.000
Average ring size = 5.8462
